LMucko/crystallography-open-database huggingface dataset:
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 80.0 GPa using ruby-scale Note: P = 84.0 GPa using MgO-scale
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013238
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 80.0 GPa using ruby-scale
 Note: P = 84.0 GPa using MgO-scale
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.822
_cell_length_b                   3.822
_cell_length_c                   3.822
_cell_formula_units_Z            4
_cell_volume                     55.831
_database_code_amcsd             0004725
_diffrn_ambient_pressure         8e+07
_exptl_crystal_density_diffrn    4.795
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013238
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 85.0 GPa using ruby-scale Note: P = 90.1 GPa using MgO-scale
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013239
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 85.0 GPa using ruby-scale
 Note: P = 90.1 GPa using MgO-scale
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.805
_cell_length_b                   3.805
_cell_length_c                   3.805
_cell_formula_units_Z            4
_cell_volume                     55.089
_database_code_amcsd             0004726
_diffrn_ambient_pressure         8.5e+07
_exptl_crystal_density_diffrn    4.860
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013239
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 89.0 GPa using ruby-scale Note: P = 94.4 GPa using MgO-scale
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013240
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 89.0 GPa using ruby-scale
 Note: P = 94.4 GPa using MgO-scale
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.794
_cell_length_b                   3.794
_cell_length_c                   3.794
_cell_formula_units_Z            4
_cell_volume                     54.612
_database_code_amcsd             0004727
_diffrn_ambient_pressure         8.9e+07
_exptl_crystal_density_diffrn    4.902
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013240
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 96.2 GPa using ruby-scale Note: P = 102.9 GPa using MgO-scale
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013241
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 96.2 GPa using ruby-scale
 Note: P = 102.9 GPa using MgO-scale
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.773
_cell_length_b                   3.773
_cell_length_c                   3.773
_cell_formula_units_Z            4
_cell_volume                     53.711
_database_code_amcsd             0004728
_diffrn_ambient_pressure         9.62e+07
_exptl_crystal_density_diffrn    4.984
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013241
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 99.6 GPa using ruby-scale Note: P = 106.4 GPa using MgO-scale
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013242
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 99.6 GPa using ruby-scale
 Note: P = 106.4 GPa using MgO-scale
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.765
_cell_length_b                   3.765
_cell_length_c                   3.765
_cell_formula_units_Z            4
_cell_volume                     53.370
_database_code_amcsd             0004729
_diffrn_ambient_pressure         9.96e+07
_exptl_crystal_density_diffrn    5.016
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013242
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 102.4 GPa using ruby-scale Note: P = 109.4 GPa using MgO-scale
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013243
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 102.4 GPa using ruby-scale
 Note: P = 109.4 GPa using MgO-scale
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.758
_cell_length_b                   3.758
_cell_length_c                   3.758
_cell_formula_units_Z            4
_cell_volume                     53.073
_database_code_amcsd             0004730
_diffrn_ambient_pressure         1.024e+08
_exptl_crystal_density_diffrn    5.044
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013243
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 106.3 GPa using ruby-scale Note: P = 113.8 GPa using MgO-scale
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013244
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 106.3 GPa using ruby-scale
 Note: P = 113.8 GPa using MgO-scale
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.748
_cell_length_b                   3.748
_cell_length_c                   3.748
_cell_formula_units_Z            4
_cell_volume                     52.650
_database_code_amcsd             0004731
_diffrn_ambient_pressure         1.063e+08
_exptl_crystal_density_diffrn    5.085
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013244
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 111.0 GPa using ruby-scale Note: P = 118.1 GPa using MgO-scale
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013245
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 111.0 GPa using ruby-scale
 Note: P = 118.1 GPa using MgO-scale
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.738
_cell_length_b                   3.738
_cell_length_c                   3.738
_cell_formula_units_Z            4
_cell_volume                     52.230
_database_code_amcsd             0004732
_diffrn_ambient_pressure         1.11e+08
_exptl_crystal_density_diffrn    5.126
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013245
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 3.6 GPa
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013246
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 3.6 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.181
_cell_length_b                   4.181
_cell_length_c                   4.181
_cell_volume                     73.087
_cell_formula_units_Z            4
_database_code_amcsd             0004733
_diffrn_ambient_pressure         3.6e+06
_exptl_crystal_density_diffrn    3.663
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013246
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 7.4 GPa
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013247
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 7.4 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.156
_cell_length_b                   4.156
_cell_length_c                   4.156
_cell_volume                     71.784
_cell_formula_units_Z            4
_database_code_amcsd             0004734
_diffrn_ambient_pressure         7.4e+06
_exptl_crystal_density_diffrn    3.729
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013247
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 10.6 GPa
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013248
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 10.6 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.133
_cell_length_b                   4.133
_cell_length_c                   4.133
_cell_volume                     70.599
_cell_formula_units_Z            4
_database_code_amcsd             0004735
_diffrn_ambient_pressure         1.06e+07
_exptl_crystal_density_diffrn    3.792
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013248
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 13.5 GPa
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013249
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 13.5 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.114
_cell_length_b                   4.114
_cell_length_c                   4.114
_cell_volume                     69.629
_cell_formula_units_Z            4
_database_code_amcsd             0004736
_diffrn_ambient_pressure         1.35e+07
_exptl_crystal_density_diffrn    3.845
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013249
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 16.2 GPa
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013250
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 16.2 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.096
_cell_length_b                   4.096
_cell_length_c                   4.096
_cell_volume                     68.719
_cell_formula_units_Z            4
_database_code_amcsd             0004737
_diffrn_ambient_pressure         1.62e+07
_exptl_crystal_density_diffrn    3.896
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013250
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 18.9 GPa
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013251
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 18.9 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.079
_cell_length_b                   4.079
_cell_length_c                   4.079
_cell_volume                     67.867
_cell_formula_units_Z            4
_database_code_amcsd             0004738
_diffrn_ambient_pressure         1.89e+07
_exptl_crystal_density_diffrn    3.945
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013251
Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure gauge for helium pressure media Note: P = 22.8 GPa
Jacobsen, S. D.; Holl, C. M.; Adams, K. A.; Fischer, R. A.; Martin, E. S.; Bina, C. R.; Lin, J. F.; Prakapenka, V. B.; Kubo, A.; Dera, P.; American Mineralogist 93 (2008) 1823–1828; doi:10.2138/am.2008.2988

data_9013252
_publ_section_title
;
 Compression of single-crystal magnesium oxide to 118 GPa and a ruby pressure
 gauge for helium pressure media
 Note: P = 22.8 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1823
_journal_page_last               1828
_journal_paper_doi               10.2138/am.2008.2988
_journal_volume                  93
_journal_year                    2008
_chemical_formula_structural     MgO
_chemical_formula_sum            'Mg O'
_chemical_name_mineral           Periclase
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.058
_cell_length_b                   4.058
_cell_length_c                   4.058
_cell_volume                     66.825
_cell_formula_units_Z            4
_database_code_amcsd             0004739
_diffrn_ambient_pressure         2.28e+07
_exptl_crystal_density_diffrn    4.006
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9013252